| ||Format||Pages||Price|| |
|8||$46.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$46.00||  ADD TO CART|
Significance and Use
5.1 Apparent viscosity versus shear rate information can be useful in predicting pressure drops in grease distribution systems under steady-state flow conditions at constant temperature.
1.1 This test method covers measurement, in poises, of the apparent viscosity of lubricating greases in the temperature range from −54 °C to 38 °C (−65 °F to 100 °F). Measurements are limited to the range from 25 P to 100 000 P at 0.1 s−1 and 1 P to 100 P at 15 000 s−1.
Note 1: At very low temperatures the shear rate range may be reduced because of the great force required to force grease through the smaller capillaries. Precision has not been established below 10 s−1.
1.2 This standard uses inch-pound units as well as SI (acceptable metric) units. The values stated first are to be regarded as standard. The values given in parentheses are for information only. The capillary dimensions in SI units in and are standard.
1.3 WARNING—Mercury has been designated by many regulatory agencies as a hazardous material that can cause central nervous system, kidney and liver damage. Mercury, or its vapor, may be hazardous to health and corrosive to materials. Caution should be taken when handling mercury and mercury containing products. See the applicable product Material Safety Data Sheet (MSDS) for details and EPA’s website—http://www.epa.gov/mercury/faq.htm—for additional information. Users should be aware that selling mercury and/or mercury containing products into your state or country may be prohibited by law.
1.3.1 In addition, temperature measuring devices such as liquid-in-glass thermometers, thermocouples, thermistors, or platinum resistance thermometers that provide equivalent or better accuracy and precision, that cover the temperature range for ASTM thermometer 49C, may be used.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health and environmental practices and determine the applicability of regulatory limitations prior to use.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D88 Test Method for Saybolt Viscosity
D217 Test Methods for Cone Penetration of Lubricating Grease
D3244 Practice for Utilization of Test Data to Determine Conformance with Specifications
ICS Number Code 75.100 (Lubricants, industrial oils and related products)
UNSPSC Code 15121902(Grease)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D1092-12(2017), Standard Test Method for Measuring Apparent Viscosity of Lubricating Greases, ASTM International, West Conshohocken, PA, 2017, www.astm.orgBack to Top